Laser ablation .
Download Policy: Content on the Website is provided to you AS IS for your information and personal use and may not be sold / licensed / shared on other websites without getting consent from its author.While downloading, if for some reason you are not able to download a presentation, the publisher may have deleted the file from their server.
In 1995, Smalley'25 at Rice University reported the synthesis of carbon nanotubes by lasers group vaporisation. The laser vaporisation apparatus used by Smalley's group is shown in Figure 2-9. A pulsed26,27, or continuous28,29 laser is used to vaporise a graphite target in an oven at 1200 °C. The main difference between continuous and pulsed laser, is that the pulsed laser demands a much higher light intensity (100 kW/cm2 compared with 12 kW/cm2). The oven is filled with helium or argon gas in order to keep the pressure at 500 Torr. A very hot vapour plume forms, then expands and cools rapidly. As the vaporised species cool, small carbon molecules and atoms quickly condense to form larger clusters, possibly including fullerenes. The catalysts also begin to condense, but more slowly at first, and attach to carbon clusters and prevent their closing into cage structures.30
Catalysts may even open cage structures when they attach to them. From these initial clusters, tubular molecules grow into single-wall carbon nanotubes until the catalyst particles become too large, or until conditions have cooled sufficiently that carbon no longer can diffuse through or over the surface of the catalyst particles. It is also possible that the particles become that much coated with a carbon layer that they cannot absorb more and the nanotube stops growing. The SWNTs formed in this case are bundled together by van der Waals forces30.
The size of the SWNTs ranges from 1-2 nm, for example the Ni/Co catalyst with a pulsed laser at 1470 °C gives SWNTs with a diameter of 1.3-1.4 nm26. In case of a continuous laser at 1200 °C and Ni/Y catalyst (Ni/Y is 2:0.5 at. %), SWNTs with an average diameter of 1.4 nm were formed with 2030 % yield, see Figure 2-10.28
A jet of preheated (1000 °C) argon through a nozzle tip is situated close to the rotating graphite target, which contains the catalyst. The argon gas deflects the ablation plume approximately 90° away from the incident FEL beam direction, clearing away the carbon vapour from the region in front of the target. The produced SWNT soot, is collected in a cold finger. This process can be seen in Figure 2-11. The yield at this moment is 1,5 g/h, which is at 20 % of the maximum power of the not yet upgraded FEL. If the FEL is upgraded to full power and is working at 100 % power, a yield of 45 g/h could be reached since the yield was not limited by the laser power.
With this method the maximum achievable yield with the current lasers is 45 g/h, with a NiCo or NiY catalyst, in argon atmosphere at 1000 °C and a wavelength of ~3000 nm. The SWNTs produced in bundles of 8-200 nm and a length of 5-20 microns has a diameter range 1-1.4 nm.27
This method is a novel continuous, highly productive laser-powder method of SWNT synthesis based on the laser ablation of mixed graphite and metallic catalyst powders by a 2-kW continuous wave CO2 laser in an argon or nitrogen stream. Because of the introduction of micron-size particle powders, thermal conductivity losses are significantly decreased compared with laser heating of the bulk solid targets in known laser techniques. As a result, more effective utilisation of the absorbed laser power for material evaporation was achieved. The set-up of the laser apparatus is shown in Figure 2-12 29.
The established yield of this technique was 5 g/h. A Ni/Co mixture (Ni/Co is 1:1) was used as catalyst, the temperature was 1100 °C. In the soot a SWNT abundance of 20-40% w as found with a mean diameter of 1.2-1.3 nm. An HRTEM-picture of this sample is shown in Figure 2-12.